#------------------------------------------------------------------------------
#$Date: 2020-01-11 00:22:35 +0200 (Sat, 11 Jan 2020) $
#$Revision: 246661 $
#$URL: file:///home/coder/svn-repositories/cod/cif/1/55/69/1556980.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1556980
loop_
_publ_author_name
'Likhacheva, A.Y.'
'Goryainov, S.V.'
'Bulbak, T.A.'
_publ_section_title
;
 An X-ray diffraction study of the pressure-induced hydration in
 cordierite at 4-5 GPa : at 1 bar
;
_journal_name_full               'American Mineralogist'
_journal_page_first              181
_journal_page_last               186
_journal_paper_doi               10.2138/am.2013.4199
_journal_volume                  98
_journal_year                    2013
_chemical_formula_sum
'Al3.96 Fe0.42 H0.9 Mg1.57 Mn0.07 Na0.07 O18.45 Si4.98'
_chemical_name_common
'Na0.07(Mg1.57Fe0.36Mn0.07)(Al3.96Fe0.06Si4.98)O18 0.45H2O'
_chemical_name_mineral           'cordierite at 0 GPa'
_space_group_IT_number           66
_space_group_name_Hall           '-C 2 2c'
_space_group_name_H-M_alt        'C c c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   17.104(2)
_cell_length_b                   9.746(1)
_cell_length_c                   9.333(1)
_cell_volume                     1555.8(3)
_diffrn_ambient_pressure         100
_diffrn_ambient_temperature      298
_cod_data_source_file            cordierite-0GPa.cif
_cod_data_source_block           cordierite-0GPa
_cod_original_formula_sum
'Na0.07 Mg1.57 Fe0.42 Mn0.07 Al3.96 Si4.98 O18.45 H0.9'
_cod_database_code               1556980
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,-z
3 -x,-y,z
4 x,y,-z
5 -x,y,-z+1/2
6 x,-y,z+1/2
7 x,-y,-z+1/2
8 -x,y,z+1/2
9 x+1/2,y+1/2,z
10 -x+1/2,-y+1/2,-z
11 -x+1/2,-y+1/2,z
12 x+1/2,y+1/2,-z
13 -x+1/2,y+1/2,-z+1/2
14 x+1/2,-y+1/2,z+1/2
15 x+1/2,-y+1/2,-z+1/2
16 -x+1/2,y+1/2,z+1/2
loop_
_atom_site_label
_atom_site_occupancy
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_type_symbol
Mg 1.0 0.1630(10) 0.500000 0.250000 Uiso 0.008000 Mg
Si1 1.0 0.1930(10) 0.0790(10) 0.000000 Uiso 0.008000 Si
Si2 1.0 0.000000 0.500000 0.250000 Uiso 0.008000 Si
Si3 1.0 -0.1370(10) 0.2360(10) 0.000000 Uiso 0.008000 Si
Si4 1.0 0.0490(10) 0.3090(10) 0.000000 Uiso 0.008000 Si
Al 1.0 0.250000 0.250000 0.251(3) Uiso 0.008000 Al
O1 1.0 0.2470(10) 0.102(2) 0.144(2) Uiso 0.010000 O
O2 1.0 -0.1680(10) 0.081(3) 0.000000 Uiso 0.010000 O
O3 1.0 0.1230(10) 0.187(2) 0.000000 Uiso 0.010000 O
O4 1.0 0.0640(10) 0.4160(10) 0.1540(10) Uiso 0.010000 O
O5 1.0 -0.0440(10) 0.249(2) 0.000000 Uiso 0.010000 O
O6 1.0 -0.1720(10) 0.3130(10) 0.1430(10) Uiso 0.010000 O
Na 0.08(1) 0.000000 0.000000 0.000000 Uiso 0.025000 Na
Ow1 0.45(1) 0.000000 0.000000 0.250000 Uiso 0.100000 O
